- Chain transfer
- P• + XR' → PX + R'•
Chain transfer reactions reduce the average molecular weight of the final polymer. Chain transfer can be either introduced deliberately into a polymerization (by use of a chain transfer agent) or it may be an unavoidable side-reaction with various components of the polymerization. Chain transfer reactions occur in most forms of addition polymerization including radical polymerization, ring-opening polymerization, coordination polymerization, and cationic addition polymerization.
Chain transfer reactions are usually categorized by the nature of the molecule that reacts with the growing chain.
- Transfer to chain transfer agent. Chain transfer agents have at least one weak chemical bond, which therefore facilitates the chain transfer reaction. Common chain transfer agents include thiols, especially DDM, and halocarbons such as carbon tetrachloride. Chain transfer agents are sometimes called modifiers or regulators.
- Transfer to monomer. Chain transfer to monomer may take place in which the growing polymer chain abstracts an atom from unreacted monomer existing in the reaction medium. Because, by definition, polymerization reactions only take place in the presence of monomer, chain transfer to monomer determines the theoretical maximum molecular weight that can be achieved by a given monomer. Chain transfer to monomer is especially significant in cationic addition polymerization and ring-opening polymerization.
- Transfer to polymer. Chain transfer may take place with an already existing polymer chain, especially under conditions in which much polymer is present. This often occurs at the end of a radical polymerization when almost all monomer has been consumed. Branched polymers are formed as monomer adds to the new radical site which is located along the polymer backbone. The properties of low-density polyethylene are critically determined by the amount of chain transfer to polymer that takes place.
- Transfer to solvent. In solution polymerization, the solvent can act as a chain transfer agent. Unless the solvent is chosen to be inert, very low molecular weight polymers (oligomers) can result.
Chain transfer was first proposed by Taylor and Jones in 1930. They were studying the production of polyethylene from ethylene and hydrogen in the presence of ethyl radicals that had been generated by the thermal decomposition of (Et)2Hg and (Et)4Pb. The observed product mixture could be best explained by postulating "transfer" of radical character from one reactant to another.
Flory incorporated the radical transfer concept in his mathematical treatment of vinyl polymerization in 1937. He coined the term "chain transfer" to explain observations that, during polymerization, average polymer chain lengths were usually lower than predicted by rate considerations alone.
The first widespread use of chain transfer agents came during World War II in the US Rubber Reserve Company. The "Mutual" recipe for styrene-butadiene rubber was based on the Buna-S recipe, developed by I. G. Farben in the 1930s. The Buna-S recipe, however, produced a very tough, high molecular weight rubber that required heat processing to break it down and make it processable on standard rubber mills. Researchers at Standard Oil Development Company and the U. S. Rubber Company discovered that addition of a mercaptan modifier to the recipe not only produced a lower molecular weight and more tractable rubber, but it also increased the polymerization rate. Use of a mercaptan modifier became standard in the Mutual recipe.
Interestingly, although German scientists had become familiar with the actions of chain transfer agents in the 1930s, Germany continued to make unmodified rubber to the end of the war and did not fully exploit their knowledge.
Throughout the 1940s and 1950s, progress was made in the understanding of the chain transfer reaction and the behavior of chain transfer agents. Snyder et al. proved the sulfur from a mercaptan modifier did indeed become incorporated into a polymer chain under the conditions of bulk or emulsion polymerization. A series of papers from Mayo (at the U.S. Rubber Co.) laid the foundation for determining the rates of chain transfer reactions.
In the early 1950s, workers at DuPont conclusively demonstrated that short and long branching in polyethylene was due to two different mechanisms of chain transfer to polymer. Around the same time, the presence of chain transfer in cationic polymerizations was firmly established.
The nature of chain transfer reactions is currently well understood and is given in standard polymerization textbooks. Since the 1980s, however, a particularly active area of research has been in the various forms of free radical living polymerizations including catalytic chain transfer polymerization, RAFT, and iodine transfer polymerization. In these processes, the chain transfer reaction produces a polymer chain with similar chain transfer activity to the original chain transfer agent. Therefore there is no net loss of chain transfer activity.
- ^ IUPAC, Compendium of Chemical Terminology, 2nd ed. (the "Gold Book") (1997). Online corrected version: (2006–) "chain transfer".
- ^ Flory, P. J. Principles of Polymer Chemistry, Cornell University Press, Ithaca, NY, 1953, p. 136. ISBN 0-8014-0134-8
- ^ Taylor, H. S.; Jones, W. H. J. Amer. Chem. Soc., 1930, 52, 1111.
- ^ Flory, P. J. J. Amer. Chem. Soc., 1937, 59, 241.
- ^ Synthetic Rubber, Whitby, G. S., ed., John Wiley, NY 1954, p. 243.
- ^ For example, Meisenburg, K.; Dennstedt, I.; Zaucker, E. US Pat. 2,321,693 (assigned to I. G. Farben).
- ^ Snyder, H. R.; Stewart, J. M.; Allen, R. E.; Dearborn, R. J. J. Amer. Chem. Soc., 1946, 68, 1422.
- ^ Mayo, F. R. J. Amer. Chem. Soc., 1943, 65, 2324.
- ^ Gregg, R. A.; Mayo, F. R. J. Amer. Chem. Soc., 1948, 70, 2372.
- ^ Mayo, F. R.; Gregg, R. A.; Matheson, M. S. J. Amer. Chem. Soc., 1951, 73, 1691.
- ^ see Roedel, M. J. J. Amer. Chem. Soc., 1953, 75, 6110 and following papers.
- ^ Overberger, C. G.; Endres, G. F. J. Polym. Sci., 1955, 16, 283.
Wikimedia Foundation. 2010.
Look at other dictionaries:
chain transfer — grandinės perdava statusas T sritis chemija apibrėžtis Aktyviojo centro perėjimas į su juo susidūrusią neaktyviąją molekulę grandininės reakcijos metu. atitikmenys: angl. chain transfer rus. передача цепи … Chemijos terminų aiškinamasis žodynas
Chain transfer gripper set — Комплект захватов цепного (листо)передающеголистопередающего¦передающего транспортёра … Краткий толковый словарь по полиграфии
Chain transfer system — Цепная (листо )передающаялисто передающая¦передающая система … Краткий толковый словарь по полиграфии
Reversible Addition Fragmentation and Chain Transfer Polymerization — Die sogenannte RAFT oder Reversible addition–fragmentation chain transfer (Reversible Additions Fragmentierungs Kettenübertragungs) – Polymerisation ist eine spezielle Form der lebenden / kontrollierten freien radikalischen Polymerisation. RAFT… … Deutsch Wikipedia
Reversible Addition Fragmentation Chain Transfer — La Reversible Addition Fragmentation Chain Transfer (RAFT) est une technique de polymérisation radicalaire contrôlée découverte en 1998 grâce à une collaboration entre la société DuPont et l équipe du CSIRO dirigée par le Pr. Ezio Rizzardo. Au… … Wikipédia en Français
Reversible Addition Fragmentation Chain Transfer Polymerization — Die sogenannte RAFT oder Reversible addition–fragmentation chain transfer (Reversible Additions Fragmentierungs Kettenübertragungs) – Polymerisation ist eine spezielle Form der kontrollierten freien radikalischen Polymerisation. RAFT wurde… … Deutsch Wikipedia
Chain growth polymerisation — Chain growth polymerization is a polymerization technique where unsaturated monomer molecules add on to a growing polymer chain one at a time . It can be represented with the chemical equation: where n is the … Wikipedia
Chain reaction — This article is about chain reactions in chemistry and physics. For other uses, see Chain reaction (disambiguation). A chain reaction is a sequence of reactions where a reactive product or by product causes additional reactions to take place. In… … Wikipedia
Chain termination — For the DNA sequencing method, see DNA sequencing#Chain termination methods. Chain termination is any chemical reaction that ceases the formation of reactive intermediates in a chain propagation step in the course of a polymerization, effectively … Wikipedia
Transfer pricing — refers to the pricing of contributions (assets, tangible and intangible, services, and funds) transferred within an organization. For example, goods from the production division may be sold to the marketing division, or goods from a parent… … Wikipedia